Electrospinning of Polymeric Nanofibers for Tissue ... · PDF file plications of...
Embed Size (px)
Transcript of Electrospinning of Polymeric Nanofibers for Tissue ... · PDF file plications of...
ELECTROSPINNING HAS GAINED POPULARITY in the last10 years due in large part to an increased interest in nanoscale properties and technologies. This technique al- lows for the production of polymer fibers with diameters varying from 3 nm to greater than 5 �m.1 Potential ap- plications of electrospinning include filtration mem- branes, catalytic nanofibers, fiber-based sensors, and tis- sue engineering scaffolds.1–3
One attractive feature of electrospinning is the sim- plicity and inexpensive nature of the setup; the typical electrospinning setup consists of a syringe pump, a high voltage source, and a collector (Fig. 1). During the elec- tro spinning process, a polymer solution is held at a nee- dle tip by surface tension. The application of an electric field using the high-voltage source causes charge to be in- duced within the polymer, resulting in charge repulsion within the solution. This electrostatic force opposes the sur- face tension; eventually, the charge repulsion overcomes the surface tension, causing the initiation of a jet. As this jet travels, the solvent evaporates and an appropriate col- lector can be used to capture the polymer fiber. Figure 2A shows a scanning electron microscopy image of an elec- trospun polymer mesh.4,5 This approach has been used suc- cessfully to spin a number of synthetic and natural6–10 poly- mers into fibers many kilometers in length.3,5
Recently, electrospinning has gained popularity with the tissue engineering community as a potential means of producing scaffolds. The objective of this review is to describe briefly the theory behind the technique, exam- ine the effect of changing the process parameters on fiber morphology, and discuss the application and impact of electrospinning on the field of tissue engineering.
THEORY OF ELECTROSPINNING
The stable electrospinning jet was described in detail by Reneker and Chun as being composed of four regions: the base, the jet, the splay, and the collection.5 In the base region, the jet emerges from the needle to form a cone known as the Taylor cone. The shape of the base depends upon the surface tension of the liquid and the force of the electric field; jets can be ejected from surfaces that are essentially flat if the electric field is strong enough. Charging of the jet occurs at the base, with solutions of higher conductivity being more conducive to jet forma- tion.5 Electric forces then accelerate and stretch the poly- mer jet, causing the diameter to decrease as its length in- creases. Additionally, solvents with high vapor pressures may begin to evaporate, causing a decrease in jet diam- eter and velocity.5 In the next region, Reneker and Chun hypothesized that radial charge repulsions cause the jet
TISSUE ENGINEERING Volume 12, Number 5, 2006 © Mary Ann Liebert, Inc.
Electrospinning of Polymeric Nanofibers for Tissue Engineering Applications: A Review
QUYNH P. PHAM,* UPMA SHARMA, Ph.D.,* and ANTONIOS G. MIKOS, Ph.D.
Interest in electrospinning has recently escalated due to the ability to produce materials with nanoscale properties. Electrospun fibers have been investigated as promising tissue engineering scaf- folds since they mimic the nanoscale properties of native extracellular matrix. In this review, we ex- amine electrospinning by providing a brief description of the theory behind the process, examining the effect of changing the process parameters on fiber morphology, and discussing the potential ap- plications and impacts of electrospinning on the field of tissue engineering.
Department of Bioengineering, Rice University, Houston, Texas. *These two authors contributed equally to this work.
to “splay” into many small fibers of approximately equal diameter and charge per unit length.5 The final diameter of the electrospun fibers upon collection is dependent upon how many splays are created.5
Rutledge and co-workers have recently used high- speed photography with exposure times as low as 18 ns to demonstrate that the jet that appears to splay is actu- ally a single, rapidly whipping jet.11,12 At high electric fields after traveling a short distance, the jet becomes un- stable, begins to whip with a high frequency, and under- goes bending and stretching.11 The group modeled the behavior of the jet in terms of three instabilities: the clas- sical Rayleigh instability and two “conducting” modes. The axisymmetric Rayleigh instability is dominated by surface tension and is suppressed at high electric fields or charge densities.11 The conducting modes are inde- pendent of surface tension and are dominated by electric forces; one conducting mode is axisymmetric and the other is nonaxisymmetric (whipping instability).11,13,14
Rutledge and co-workers examined the competition be- tween these instabilities for various applied electric fields and the flow rate and determined the dominant mode.11
They constructed operating diagrams that outlined the conditions at which whipping could be expected; their predictions agreed well with experimental results.11
PARAMETERS OF ELECTROSPINNING PROCESS
From the previous description of theory, it is clear that the electrospinning process can be manipulated by a num- ber of variables. Doshi and Reneker classified the pa- rameters that control the process in terms of solution properties, controlled variables, and ambient parameters.4
Solution properties include the viscosity, conductivity, surface tension, polymer molecular weight, dipole mo- ment, and dielectric constant. The effects of the solution properties can be difficult to isolate since varying one pa- rameter can generally affect other solution properties (e.g., changing the conductivity can also change the vis- cosity). Controlled variables include the flow rate, elec- tric field strength, distance between tip and collector, nee- dle tip design, and collector composition and geometry. Ambient parameters include temperature, humidity, and air velocity. In this section, studies that investigate the effect of each parameter on electrospun fiber morpholo- gies and sizes are highlighted.
Solution viscosity (as controlled by changing the poly- mer concentration) has been found to be one of the biggest determiners of fiber size and morphology when spinning polymeric fibers. The relationship between the
PHAM ET AL.
polymer viscosity and/or concentration on fibers obtained from electrospinning has been studied in a number of sys- tems,15–25 including poly(DL-lactic acid) (PDLA),15
poly(lactic-co-glycolic acid) (PLGA),16 poly(ethylene oxide) (PEO),9,17–19 poly(vinyl alcohol) (PVA),20–23
poly(methyl methacrylate) (PMMA),24 polystyrene,25
poly(L-lactic acid) (PLLA),26 gelatin,6 dextran,8 and col- lagen type I-PEO.9 At low polymer concentrations, defects in the form of beading and droplets have been observed (Fig. 2B);6,8,9,15,17,19,21,22,25,27–33 the process under these conditions was characteristic of electrospray- ing rather than spinning.28 Additionally, the presence of junctions and bundles have been seen, indicating that the fibers were still wet when reaching the collector.17 In- creasing the solution viscosity by increasing polymer con- centration yielded uniform fibers with few beads and junc- tions.6,9,17,25 In some cases, increasing the concentration of a polymer solution can also affect its surface tension;17
however, for polystyrene solutions with constant surface tension, beading still decreased with increased viscosity.25
This result indicates that the variation in viscosity was re- sponsible for the morphological change of the fibers.25 For solutions that were too concentrated (and therefore too vis- cous), the droplet dried out at the tip before jets could be initiated, preventing electrospinning.15,28,34
Attempts have been made to quantify the minimum polymer concentrations and viscosities required to elec- trospin fibers. Koski et al. found that it was possible to spin PVA as long as [�]c � 5 where [�] was the intrin- sic viscosity and c was the concentration.20 For PEO, it was found that solutions with [�]c � 10 allowed for spin- ning.18 McKee et al. found that a concentration greater than the entanglement concentration, ce, was required to spin linear and branched poly(ethylene terephthalate-co- ethylene isophthalate) (PET-co-PEI).35 Solutions with concentrations 2-2.5 times the entanglement concentration yielded uniform, bead-free fibers.35 Recently, Gupta et al. synthesized PMMA and determined the critical chain over- lap concentration, c*.24 They determined that when the so- lution concentration was less than c* there was insufficient chain overlap to form polymer fibers; at all conditions, droplet formation was observed.24 In the semi-dilute re- gion (concentrations between c* and ce), beading was oc- casionally observed. At concentrations approximately dou- ble ce, uniform, bead-free fibers were obtained.24
The diameter of the fibers produced by electrospinning has been found to increase with increasing solution con- centration.6,17,35–37 For example, PLLA fibers with di- ameters of 100-300 nm were produced from 1 wt% so- lutions while 5 wt% solutions yielded 800-2400 nm fibers.26 Additionally, the diameter of PVA fibers in- creased from 87 � 14 nm to 246 � 50 nm by increasing the PVA concentration from 6 to 8%.21 It was found that an increased fiber diameter correlated directly to a de- crease in the surface area of electrospun mats.37
Researchers have aimed to find a relationship between solution concentration and the fiber diameter. For exam- ple, it was found that increasing the concentration of gelatin yielded fibers wit